● Polymer Blends
1. Polymer-polymer Miscibility
By Olabisi, Robeson, and Shaw
2. Poplymer Blends, by D.R Paul, Ed,
Academic Press (1978).
3. specific Interactions and the Miscibility of Polymer
by Coleman, Graf, and Painter(1990)
4. Polymer Alloys and Blends, Thermodynamics and
Rheology, by L.A. Utracki,(1990).
● Blend Preparation 방법:
(a) Melt blending- screw extruder를 사용하여 blend하고자 하는
고분자를 용융점 이상에서 extrusion하여 mixing함.
(b) Solution blending- mixing하고자 하는 고분자의 cosolvent를
사용하여 solution으로 만든 다음 cast하여 필름(film) 상태
로 blend를 제조함.
(ex) polymer membrane(분리막)제조시.
그러나, amorphous polymer와 crystalline polymer를 blend했을때
는 film의 투명성으로부터 사용성을 판별하기는 어렵다.
(2)DSC(differential scanning calorimetry):
시차 주사 열분석기를 이용하여 블렌드의 Tg(유리전이 온도)를 측
정함으로서 상용성을 관찰함-가장 많이 쓰이는 방법중 하나임. 즉
(i) a single phase exhibits one Tg.
(ex) A polymer : Polycarbonate, Tg=150°C (423 K)
B polymer : Polycaprolactane, Tg=-52°C (221 K)
Blend (A+B)/50:50인 경우
BlendTg (TgBlend=17.3°C (290.3 K)
(2) microscopy method (Scanning Electron microscopy).
(3) FT-IR (Fourier Transform IR)
(4) Ternary solution method (polymer 1- polymer 2 - solvent)
- Compatible components from a single, transparent phase in
mutual solution, while incompatible polymers exhibit phase
seperation if the solution is not extremely dilute.
- Equilibrium is relatively easily achived in dilutions and
- Blends of immiscible (or partially miscible) materials can
useful so long as no significant desegration occurs while
mixture is being mixed.
● Practical Aspects of Polymer Blending.
- Polymer blends have become a very important subject for
investigation in recent years.
- Copolymerization and blending are alternative routes for
properties of polymers.
- Blending is less expensive.
- The restriction of environment pollutions.(solvent for
● Objectives in Marking Blends
- components of the mixture adhere to each other well enough to
adequate mechanical integrity for the pair.
- load bearing capacity be maintained for the expected
of the particular article.
- Miscible blends should give better mechanical properties.
(e.g) poly (phenylene oxide) and polystyrene-trade name “Noryl”
● Procedure to Retard on Eliminate Demixing.
1. Use of miscible component ( i,e, Gm = Hm – T S < 0).
(a) Low-molecular-weight polymers
(b) Specific interactions to produce negative Hm
(c) Generally match solubility parameter of Flory-Huggins
2. Rely on slow diffusion rates
(a) Mix high-molecular-weight polymers
3. Prevent segregation
(b) Forming interpenetrating polymer network(IPN)
(c) Mechanical Interlocking of components.
4. Use “compatibilizing agents”
(a) Statical copolymers
(b) Graft copolymers
(c) Block copolymers
● Procedures to Retared or Eliminate Demixing of Polymer
1.Use of Miscible Components
- Themodynamically stable mixtures will of course form
blends This implies miscibility on a molecular level.
(a) Use of low molecular-weight polymers
Gm = Hm – T Sm < 0
Increasing the entropy of mixing, Sm will favor a more negative
(e.g.) low m.w. of polystyrene and poly(methyl methacrylate) are
but high m.w > 100,000 are not.
(b) Specific interactions to produce negative Hm.
(e.g.) hydrogen-bonding, dipole-dipole interactions, acid-base
(b) specific interactions to produce negative Hm
(hydrogen-bonding, dipole-dipole interactions, acid-base
(CH2)5 C On
CH2 CH2 O CH2 CH2 O CH3 CH2 O
e.g) If specific interactions do occur between the components
a polymer blend, the mixing process will be exothermic (
< 0)and miscibility can be realized.
1. The hydrogen bonding between the α-hydrogen of the
carbonyl oxygen of poly(ε-caprolactone).
2. The phenyl group coupling between the aromatic rings of
poly(2,6-dimethyl-1,4-phenylene oxide)and polystyrene.
3. Dipole interactions in the blends of poly(vinylidene
fluoride)and poly(methyl methacrylate).
Acid - Base interactions
- SO3-Na+ + Cl-NR3 SO3
-+NR3 - + Na+Cl-
(C) Solubility parameter or Flory-Huggins interaction
• The most widely used method for predicting miscibility
mayching solubility parameters and hydrogen-bonding
• A small or negative Flory-Huggins parameter value is also
characteristics of a stable mixture.
(e.g) 1O112 (=V δχ - 2δ )
assume: Hm is derived only for the Van der Waals
Specific interactions like ionic, or htdrogen bonds are
implicitly eliminated from the model.
• Solubility parameters can be assigned a priori to the
components of a mixture, while χ values must be determined
by experiments with the actual mixture.
The χ parameter refers to a pair of components and can
include specific interactions even if they are not mentioned
the basic Flory- Huggins theory.
2. Reliance on Slow Diffusion Rates
(a) High-Molecular-Weight Polymers
- Since demixing is a diffusional process, it can be reduced
an acceptable level by using higher-molecular-weight, more
- the rate of segregation will be retarded.
-portions of each are anchored in the ordered resions in
they both participate.
(e.g) polyethylene +polypropylene+ethylene/propylene
copolymer (compatibilizing agent)
(3) Prevention of Segregation
•a thermoset system-cross-linked
• a thermoplastic system
(e,g) conductive carbon black is mixed with a peroxide,
polyethylene, rubber.-yield semiconductive polymers when
peroxide decompses it produces radicals, and the parent
polymers are linked by primary balance forces(bonds) .
(b) Interpenetrating Polymer Networks (IPN)
- IPN is formed by swelling a cross-linked polymer with a
monomer and polymerizing and cross-lingking the latter to
produce interlocked networks.
- In semi IPN systems, only the first polymer is cross
-Most of these materials reveal phase seperation but the
vary in size,shape.
and sharpness of boundaries depending on the basic
of the component polymers, the cross-link density in the two
polymers, and the polymerization method.
-A certain degree of inherent affinity of the components is
needed for ordinary IPN because they must form solutions or
swollen networks during synthesis.
-This may not be required(inherent affinity)
for IPNs based on latex polymer, where a solvent can be
to the first, cross-linked latex polymer to open it up to
penetration by the second monomer and cross-linker.
(c) Mechanical Interlocking of Components
- a blend may be prevented from demixing because of numerous
mutual entanglements produced by mechanical processing.
(e.g) If the melt viscosity of polypropylene and
terephthalate) polymers are reasonably matched under
extrusion conditions, a finely dispersed blend may be
in fiber form.
- orientation of such fibers yield strong filaments in which
microfibrils of the two partially crystallized polymers are
intertwined and unable to separate.
(4) Use of "Compatibilizing Agents"
- Mixtures of immiscible polymers can be made more stable by
addition of another material that adheres strongly to the
components of the blend.
(e.g.) poly(vinyl chloride)/poly(methyl methacrylate)
plus dioctyl phthalate, phthalate ester.
(a) statistically copolymer 사용.
(e.g) PVC/(ethylene-ethyl acrylate- carbon monoxide)
(b) Graft copolymer
(e.g.) ① high impact polystyrene(HIPS)-polystyrene with
② poly(acrylonitrile-butadiene-styrene) (ABS)
③ rubber-toughened glassy polymers polystyrene and
-grafting procedures are needed for effective rubber
of relatively brittle glassy
polystyrene and SAN.
(c) Block copolymers
-Block and graft copolymers have generally similar effects
collecting at interfaces
dispersions of one
homopolymer in another.
- graft copolymers-made by free-radical process.
block copolymers-made by ionic or step-growth process.
(e.g.) ABS type(styrene/butadiene/styrene)
• Several types of phase behavior in liquid.
Example: (a) A common one
(b) water + n-hexane
(c) water + triethylamine
(d) water + nicotine
(e) partially miscible polymer mixtures.
(e.g) polycarbonate + PET
or - polystyrene in cyclohexane.
depending on m.w. of polystyrene.
(a) upper critical solution temperature (UCST)
(b) lower critical solution temperature (LCST)
(c) UCST and LCST 공존.
• Method for Determining polymer-polymer Miscibility.
① glass transition temperatures (Tg):
- the most commonly used method for establishing miscibility
polymer-polymer blends or partial phase mixing.
- a miscible polymer blend will exhibit a single glass
between the Tg's of the components while for partially
systems the Tg's approach each other but do not become
- differential scanning calorimetry (DSC)
- mechanical method using dynamic mechanical thermal
: the slastic and viscoelastic properties of polymers derived
subjecting polymers to small-amplitude cyclic deformation
yield important information concerning transitions occurring
(tanδ vs temp.)
- Direct visual confirmation of the presence of two phases.
- Heterogeneities exist in miscible polymer systems by
- Phase contract microscopy: require as a minimum a
refractive index between the phases for contrast.
- Electron Microscope : transmission electron
been widely used in polymer-polymer studies.
• the necessary step of microtoming (500oA ) can be facilitated
(e.g.) SBR-PB (Styrene-Butadiene rubber)and (Polybutadiene)
• scanning electron microscopy(SEM) is very useful in
(cross-section) studies of polymer blends.(need gold
about 400oA )
③ Scattering Methods.
-cloud-point curve (CPC) : the CPCs found on heating and on
LCST found polystyrene-poly(vinyl methyl ether).
poly(vinylidene fluoride)- PMMA
• light scattering : sensitive to density and concentration
• X-ray scattering: sensitive to density fluctuations.
• Neutron scattering : measures the differential Neutron
cross section of small concentrations of protonated polymer
dispersed in a matrix of deutrerated polymer.
-by allowing the polymer-polymer-solvent mixture to stand,
for a few days, if phase seperation does occur the two
said to be immiscible.
(a) when two high polymers are incompatible in one solvent,
are generally also incompatible in all other solvents, but it is
(b) the limit of phase seperation depends on the nature of
(c)the molecular weight of the polymers is of great
(d)there is no obious relationship between the compatibility of
two polymers and the chemical nature of their monomers.
⑤melting point (Tm) depression method :
−V : molar volume.
0fHΔ : perfect crystal heat of fusion.
0mT : equilibrium melting point
blendmT : equilibrium melting point in the blend.
Subscript 1 for amorphous polymer, 2 for crystalline
1. Nish & Wang, Macromolecules 8,909 (1975).
2. Rostami, Polymer, 31, 899(1990).
⑥ Inverse Gas Chromatography Method (IGC).
- traditional gas chromatography determines the property of
unknown sample in the moving phase with a known stationary
phase, while the inverse method determines the property of
stationary phase with the aid of a known vaporizing solute in
- in operation, the polymer material is placed in the column
maintained at a temperature which is at least 50°C above the
system Tg for glassy material and Tm for a crystallizable
(e.g.) ① poly(vinyl chloride) - Dioctyl phthalate by IGC,
Patterson, and Schreiber.
(ref.) J. Appl. Polym.Sci., 20,1025 (1976)
② PVC- poly(ε-carolactone)(PCL),
O.Olabisi, Macromolecules,8,316 (1975)
• Polymer mixing 방법:
i) screw extrusion
ii) solution casting / precipitation
iii) freeze drying etc.
- screw extruder 사용 시 측정할 수 있는 polymer melt properties.
• melt density of mixture:
σ + 22
• apparent shear rate(•γ )측정:
where Q is the volumetric flow.
R is the radius of the die.
• apparent shear stress (τ)
P is the measured pressure.
R is the die length.
• Extrudate swell ratio.
= (diameter of the extrudate)/(diameter of the capillary)